C 2 Planning resources for Sheet 75 Coating materials on PVC base on hot dip galvanised steel (PVC) General description of material: one-component coating material Binders: ZB and DB: vinyl chloride copolymer (PVC) Pigments: ZB and DB: micaceous iron oxide, tone pigments Solvent content: maximum 45 % Thinner: substance No 675.99; maximum 5 % addition Additional notes: object temperature at least 5 °C and at least 3 K above dew point Table C 4.3.2: Planning resource for materials according to Sheet 75 Area of application Protective system Application Minimum waiting time before System Surface Nominal dry film thicknesses subsequent structure preparation [μm] coating at approx. 20 °C dry wet Hot dip galvanised Hot dip Be ) hot dipping none steel structures like: galvanising as per DIN EN ISO - railings 1461) - doors ZB: 1K-PVC-EG clean 100) 240 Spraying, 8 h - inspection No depending spreading, trolleys, 675.61 to on the rolling) - inspection 675.74) surface catwalks, condition and - drainage pipes, dirt - signal gantries DB: 1K-PVC-EG and brackets subst. No - railway platform 675.61 to roof structures. 675.743,4) Materials according to 75 are not suitable: for prolonged contact with water, − for high mechanical stress, e.g. gratings − for objects at risk of fire −
C 2 Planning resources for Sheet 75 Coating materials on PVC base on hot dip galvanised steel (PVC) General description of material: one-component coating material Binders: ZB and DB: vinyl chloride copolymer (PVC) Pigments: ZB and DB: micaceous iron oxide, tone pigments Solvent content: maximum 45 % Thinner: substance No 675.99; maximum 5 % addition Additional notes: object temperature at least 5 °C and at least 3 K above dew point Table C 4.3.2: Planning resource for materials according to Sheet 75 Area of application Protective system Application Minimum waiting time before subsequent coating at approx. 20 °C System structure Surface preparation Nominal dry film thicknesses [μm] dry wet Hot dip galvanised steel structures like: - railings - doors - inspection trolleys, - inspection catwalks, - drainage pipes, - signal gantries and brackets - railway platform roof structures. Hot dip galvanising as per DIN EN ISO 1461) Be ) hot dipping none ZB: 1K-PVC-EG No 675.61 to 675.74) clean depending on the surface condition and dirt 100) 240 Spraying, spreading, rolling) 8 h DB: 1K-PVC-EG subst. No 675.61 to 675.743,4) Materials according to 75 are not suitable: − for prolonged contact with water, − for high mechanical stress, e.g. gratings − for objects at risk of fire
text_2011_0574_D.docx